Upload
others
View
3
Download
0
Embed Size (px)
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
1
Young’s modulus of tungsten at elevated temperatures using
synchronous laser shadow vibrometry
H. S. Ayoub1, Ashraf F. El-sherif
2 , H. H. Hassan
3, S. A. Khairy
4
1, 3, 4 Department of Physics, Faculty of Science, Cairo University, Egypt
2Laser Photonics Research Center, Engineering Physics Department,
Military Technical College, Cairo, Egypt
Abstract:
This paper presents the use of an improved laser shadowgraphy method for measuring
the dynamic elastic moduli of tungsten, from room temperature to near melting point. The
method is based on measuring the frequency of impulse induced longitudinal vibration of a
tungsten filament, subject to joule heating. The natural resonance frequency of the filament is
obtained by lock-in synchronous photo-detection of the laser generated filament
shadowgraph. The correlation between the filament natural frequency and its temperature
lead to the calculation of shear modulus at variable temperatures, the tensile and bulk
modului of tungsten. The results were compared to those obtained by laser Doppler
vibrometry of a tungsten wire induced by pulsed current technique. Our method permitted a
wider measuring temperature range and an easier calculation procedure. The used setup was
simple, non-destructive, non-contacting and accurate, enabling low cost vibrometry
measurements that help in future synthesis and test of new grades of refractory materials,
deployed as plasma facing material in the latest fusion reactor or super alloys in critical
applications.
Keywords:
Tungsten, elasticity moduli, elevated temperatures, , shadowgraphy, laser
vibrometry, lock-in amplifier, low cost.
Background
As the demand for tungsten and its alloys in engineering and experimental nuclear physics
continue to grow, the need for performing more accurate thermo-mechanical testing also
increases [1-10]. The most required metallurgic characteristic in this context is the elevated
temperature dynamic elasticity [11-13] that helps in developing advanced metallic grads of
refractory materials [14-18]. Many technique were developed to measure the dynamic elastic
moduli [19-21] but fewer is suitable for elevated temperatures [22-41]. One of the prominent
technique used to measure the dynamic young’s modulus of tungsten at high stresses and
temperatures, is the laser Doppler vibrometry of a wire sample induced by high current pulses
[23]. This technique enable measurements in the range from room temperature to 2650 C.
A second order parametric equation is used for fitting the experimentally obtained Young’s
modulus data over the mentioned thermal range on the form:
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
2
( ) (1)
Where ao, a1 and a2 are the regression constants. This result was achieved using a number of
sophisticated equipment ( such as laser Doppler vibrometer, spectrum analyzer, high-
resolution pyrometer...) and through a complex procedure. This procedure is based on
calculating E at a certain temperature T as an equivalent tensile modulus function on the
form:
( ) ( ( ) ( ) ( ) ( )) (2)
Where is radial frequency of the vibrating wire (depends on wire length l and the vibration
mode n), is its radius, is its material density is the Poisson ratio and is the root of
Bessel function. Only two parameters in this method were obtained experimentally, those
parameters are f and T. the rest are obtained through parameterization of published and
reference data, characterizing tungsten. Moreover, T is another implicit function or:
( ( ) ( ) ) (3)
Where the equivalent temperature function, is the emissivity of the wire surface at
measured temperature (depends on surface roughness ), the electric current pulse intensity
pulse duration and repetition rate .
Figure 1. Block diagram representing the measurement of the dynamic Young’s modulus of a tungsten wire
using laser Doppler vibrometry and pulse current heating technique [23]
So many sources of error are involved in this procedure, where the most important are those
based on temperature calibration and non-linear thermal distribution along the wire sample,
caused by clamps thermal cooling or “end-loss” [42-47]. Table 1. Shows a summary of the
error sources in this procedure
Table 1. Summary of the error sources in LDV- pulse current heating technique
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
3
The error Origin of the error effect on the
measurements
Radial velocity and radial
displacement conversion errors. Processing errors.
Thermal expansion of the wire cross-section.
Low
High temperature calibration error in
LDV LDV bad response due to optical saturation at
elevated temperature measurement.
Laser speckle noise. [48, 49]
High
Absolute temperature calibration error
in pyrometer Sample roughness and variable emissivity as a
function of temperature changes.
Optical absorption through cavity windows.
Slow response of pyro-detector vs. thermal pulses.
High
End-loss cooling error Thermal distribution gradient due to thermal
cooling of the wire sample through clamps. [43]
Very high
Nonlinear vibration modes and
frequency error Vibrational multi-degree of freedom due to
nonlinear elasticity distribution along the wire
sample in analogy to the thermal gradient.
Friction with the feed through end.
Moderate
Linear expansion error Variation in the wire sample cross-section. Low
Parametric approximation in
temperature variant inputs (i.e.
emissivity, density and Poisson ratio)
Various data for the same material grade. Low
In this work, we reported a method for measuring the elastic moduli of tungsten at elevated
temperatures with good accuracy, excluding the error caused by transient heating and thermal
gradient. We propose in this contest to change the shape of the sample from straight wire to
coiled filament, to make use of the shading factor discovered by Langmuir at the beginning of
the last century [47]. He proved that the thermal gradient of the coiled tungsten wire, is lower
than that of the straight wire [42]. We believe that such change should also ease the
measurement procedure by decreasing the resonance frequency of the sample and excluding
the higher vibration modes.
Theory of the measurement
The fundamental transverse vibration frequency of a wire string is calculated from the
equation
√
(4)
If the same string wire is reformed and coiled to form a fixed-fixed end compression spring
(as seen in figure 2) of wire diameter d , coil diameter D, number of turns N and wire
material shear modulus G, then, the frequency of the fundamental longitudinal vibration is
given by the equation [50]:
√
(5)
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
4
(a) (b)
Figure 2. Changing the symmetry of the sample from (a) String wire with transvers vibration, to (b) Helical
coil with longitudinal vibration.
Dividing equation 5 by equation 4 to obtain the frequency ratio for both string and coil
symmetry,
√
(6)
But E and G are both related by the Poisson ratio equation given by [51];
𝜐 (
) (7)
Replacing E and G in equation 6 by their value in equation 7 we obtain:
√ ( ) (8)
However, the length of the coil wire can be approximated as a sum of the perimeters of N
circular turns to obtain:
(9)
Replacing equation 9 in equation 8 to obtain:
√ ( ) (10)
Let μ representing the spring index of the helical spring like sample
(11)
By replacing equation 11 in equation 10 and assuming υ = 0.28 to obtain
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
5
(12)
If we choose μ = 4 , we conclude that and the resonance frequency of the
spring is at least one order of magnitude lower than the frequency of the equivalent string.
This result will ease the measurement as well as it will exclude all sophisticated instruments
from the test that will directly yields the shear modulus of the sample as given by the
following equation obtained from equation 5:
( ) ( ) (
)
(13)
The density of the sample as a function of temperature is given by the parametric equation
[23]:
( ) kg.oC.m
-3 (14)
Once G(T) is obtained, E(T) and K(T) representing the bulk modulus can be easily calculated
from the Poisson ratio relations as follows:
( ) ( ) [𝜐( ) ] (15)
and
( ) ( ) [ ( ) ]
[ ( )] (16)
Also, the Poisson ratio of tungsten is obtained from the parametric equation [23]:
𝜐( ) (17)
Using the formalism of exponents [52], the temperature T of incandescent tungsten coil as a
function of it electric resistance R is calculated from the equation:
(
) (18)
Where To and Ro represent the room temperature and room temperature resistance of the
sample. If we replace To by 2 C and R by the voltage difference applied on the sample V
divided the current passing through its terminals I we obtain:
[ (
) ] (19)
Now we are ready to measure the elastic moduli of tungsten as a function of temperature
using only current, voltage and frequency readings, under the effect of mechanical impulse
excitation. To retrieve natural vibration frequency data for the incandescent coil, we replaced
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
6
Doppler vibrometry by laser shadowgraphy, where vibrometry is applied on sample’s shadow
using a simple optical setup. (Figure 3 shows the block diagram of our proposed method)
Figure 3. block diagram representing the measurement of the dynamic Young’s modulus of a tungsten filament
using laser shadow-vibrometry and DC current heating technique.
As mentioned before, we introduced an new idea in shadowgraphy, by using synchronous
optical detection under lock-in condition. This improvement enable to exclude laser speckles
changes in the shadowgraph background from being detected as popcorn noise. the setup is
then able to detect very small shifts in dark shadows positions even in the presence of noisy
optical background such as artificial lighting and self-incandescence of the sample, with
detection sensitivity approaching 60dB. If the filament is placed in the focal plane of the
throw lens of focal length Df , then, the shadowgraph of the filament is projected on the
photo-detector at throw distance DT With magnification factor X given by the equation:
(20)
If the filament undergoes a small in-plane position shift due to vibration, then this shift will
be magnified at the shadowgraph plan by a factor of X . This method can detect small shifts
as 1×10-7
m assuming that X ≤ 2000× and knowing that the theoretical limit is in order of
1×10-8
m [53]. The amplitude of the lock-in output signal is proportional to the magnitude of
laser intensity changes at the object’s shadow bright/dark boundaries. In order to maximize
the output signal, the laser source intensity should be adjusted to bring the photo-detector
below saturation. In addition, it is important to place the detector window center at the
boundary between the object’s shadow and the background laser illumination at the
shadowgraph plane. The resulting vibration pattern after one mechanical pulse that is
required to excite the free natural resonance of the filament sample may be illustrated by a
damping oscillation pattern as shown in figure 4.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
7
Figure 4 . Free vibration pattern of elastic solids by pulse excitation technique
where the amplitude A of the oscillation at any time t after excitation, is given by the
equation:
( ) ⁄ (21)
τ is the time interval between A and A/e. This time interval depends on the internal friction
of the sample that may represented by the inverse of the oscillation quality factor given by the
expression [13];
(22)
( )
( ) ⁄ ⁄ (23)
Where. T is the period of one oscillation of frequency f. Hence, we can obtained Q-1
graphically from the impulse excitation pattern of the helical filament sample, the relation
between the temperature and the internal friction of tungsten shall be revealed. The frequency
spectrum of the resonance pattern may be obtained by fast Fourier transforms (FFT). Finally,
our method has several major advantages over the pulsed current method. Table 2.
summarizes the major parametric differences between laser Doppler vibrometry method and
our laser shadow-vibrometry method for measuring the dynamic Young’s modulus of
tungsten at elevated temperatures.
Table 2. Parametric comparison between laser Doppler vibrometry and laser shadow-vibrometry method
Parameter Doppler vibrometry method laser shadowgraphy based-
vibrometry method
Tungsten sample form Wire sample Coiled sample
Sample mass 10-3 - 10-2 kg 10-5 - 10-4 kg
Sample preparation Intensive Extensive
Heating current type Pulsed current Direct current
Current intensity 103 Amperes few Amperes
Temperature measurement Pyrometer Absolute calibration
Mechanical excitation method Electric pulse Mechanical shock
Pulse shape Non- Gaussian Gaussian
Frequency detection Laser Doppler vibrometry Laser shadow- vibrometry
Detected phenomena Laser frequency changes Laser intensity variations
Phenomena causality wire radial velocity changes Coil shadow position changes
FFT signal analysis Complex Simple
Harmonic autocorrelation test complex Simple
Temperature gradient High Low
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
8
Frequency range Ultrasound Audio
Setup cost High Low
Optical noise rejection Low Very high
Detector saturation Very high Very low
Room temperature elasticity Only possible Measurable
Measured parameter Young’s modulus Shear modulus
Measurements range Up to 2 0 c Up to 3400 c
Cooling Yes No (due small sample mass)
Power Consumed High Low
Sample surface roughness Essential Not Essential
Internal friction measurements Not possible Possible
Magnitude of Impulse force Not controllable Controllable
Direction of impulse force Not selectable Selectable
Type of the impulse force Thermal gradient elastic reaction Pure mechanical shock
Vibration mode control Not possible Possible
Experimental work
(a) (b) (c)
Figure 5. Experimental tungsten filament of 12 volt lamp (a) BA15 standard stop & flasher lamp blueprint (b)
The basic lamp parts (c) Magnified view of the internal helical filament and its supports.
We designed a simple setup to prove the concept of measurement and to test its accuracy, so
we decided to use commercial grade non-sag tungsten (99% purity) as test material basically
used in incandescent lamps. We searched then for the best lamp with nearly ideal geometry
and power that met our requirements. We selected a cheap P21W12V automotive
incandescent lamp previously studied in many works before [54-60]. This lamp still in
production and still sold in worldwide market. As shown in Figure 5.a, the selected lamp is
compact, lightweight and has a nearly-spherical transparent glass envelope that permits laser
shadowgraphy without distortion. It encloses a horizontal single coiled linear helical filament
produced by powder metallurgy (Figure 5.b). This filament is clamped to a very thick
refractory clamping supports relative to filament wire diameter which insure that their
resonance frequency is so much higher than the frequency of the filament by an order of at
least two decades. The contact surface area between the tungsten wire and the clamp is very
small leading to a high thermal resistance that keeps the support relatively cold with
comparison to the incandescent filament (Figure 5.c). The normal operating temperature of
the filament is about 2400oC, hence we shall overdrive the lamp and exceeding the operating
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
9
voltage to increase the heating current till reaching the near melting temperature of tungsten.
Table 3 summarized the basic physical parameters of lamp.
Table 2. Physical characteristics of the P21W12V automotive tungsten lamp
Room temperature parameter Symbol Value Unit
Electric resistance R 0.5 Ω
Wire material resistivity ρe 5.65×10-8
Ω m-1
Wire length l 6×10-2
m
Wire diameter d 9×10-5
m
Coil diameter D 5×10-4
m
Spring index µ 0.1 -
Coil length L 6×10-6
m
Wire mass m 1.1×10-5
kg
Wire material density ρ 19300 kg / m-3
Wire shear modulus G 1.6×1011
m-1
Filament natural frequency (longitudinal) f 1×103 Hz
Filament tungsten purity W 99.0 %
Tungsten filament potassium impurities content K 6 ppm
Lamp mass M 0.015 kg
Lamp nominal operating voltage V 12 V
Lamp nominal operating current I 1.45 A
Lamp pressure P ≤1 bar
Inert gas type Ar - -
The lamp sample is placed in a special mounting stage that permitted to a miniature 5volts
solenoid motor plunger (type SF11015) to stroke its glass envelope. Each stroke is a 5ms
Gaussian shape mechanical pulse along the filament axe that excite flexure vibration. The
base of the lamp is fixed to the body of the stage by hard thermal silicon rubber that isolates
the vibration of the lamp from the surroundings. The mounting stage enable precise position
adjustment of the sample as well as the solenoid to insure best axial alignment. All mounting
components are rigid enough to exclude their ultrasonic flexure resonance frequency from
being interfered with that of the filament during measurements.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
10
Figure 6. The sample mounting stage and its components.
If the solenoid plunger axe is perfectly aligned to the filament axe, the filament is forced to
oscillate at the desired longitudinal modes only as shown in figure 7. The gap between the
plunger and the filament must be adjusted also to yield best results. Later we discovered that
the gap width can be reduced till vanishing and the filament still excited by the minimum
solenoid plunger displacement . If the axis are misaligned then the filament shows undesired
complex modes of vibration that is eventually a mix of both transversal and longitudinal
modes.
Figure 7. Generation of filament undesired out-of-plan vibrations caused by the misalignment of the solenoid
plunger axe to the filament axe
The sample mounting stage is then placed in a laser shadowgraphy-based vibrometer setup
that we built as shown in the illustration of figure 8. This setup included a focusable 100mw
semiconductor laser (wavelength = 536nm), electrically modulated with 33 kHz square wave
carrier frequency at 90% modulation depth. The laser beam is expanded into linear beam
shape by a rod lens (diameter = 5mm). The expanded beam is backlighting a horizontally the
tungsten filament sample. The sample receives a mechanical excitation pulses from a from
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
11
solenoid motor plunger (stroke time = 5ms). A small focal length convex throw lens (focal
length = 20mm) and a pinhole filter (hole diameter = 1mm) are used to generate a
shadowgraph for vibrating filament. This shadowgraph is projected 60 cm away on a ground
glass screen in which a photo-detector window (Photodiode type BPW21) is piercing the
screen surface. The photo-detection of the filament shadow vibrations is synchronized with
the laser modulation to detect the sample resonance signal to be recorded by digital storage
oscilloscope.
Figure 8. Illustration of the setup basic optical components and instrumentation.
The setup was realized in a lightweight, compact, fast to install and easy to operate layout
(figure 9). Most instrumentation were designed and manufactured in the laboratories of the
Faculty of Science at Cairo University. The setup was also equipped by a parametric
equalizer and an audio amplifier for demonstration of audible filament resonance at different
temperatures.
Figure 9. The experimental setup and instrumentation used in this work
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
12
It is important to mention that the key of success in our measurement is the good optical
alignment so that, the filament must completely illuminated by the laser beam (figure 10a)
and the center of resulting shadowgram should be projected appropriately on the detector
window (figure 10b).
(a) (b)
Figure 10. Close-up showing (a) The optical setup during laser exposure (b) The filament shadowgraph
projected on the aiming screen on the photo-detector window.
We started the measurements by heating the filament for at least one hour at temperature of
2400oc to sinter the non-sag filament and to allow minimum dislocation defects. At the
moment of sudden heating we will notice a minor change in the filament pitch and axial
position on the screen due to thermal expansion as we verified in another work [56]. If the
alignment process concur some complications then it is recommended to exclude the pinhole
filter for a while till finishing all necessary adjustments. Figure 11 show the importance of
pinhole filter to screen the luminosity of the filament at incandescence.
(b) (b) (c)
Figure 11. (a) Magnified traveling microscope image of the tungsten filament part subjected to laser
shadowgraphy. (b) The screen projected image of the filament part at incandescence without pinhole filter. (c)
The shadowgraph of the same part of the filament at incandescence after adding the pinhole filter.
We restarted heating the filament slowly and gradually on a 50 or 100 mA increment. Each
time we activated the solenoid and recorded the yielded impulse pattern by the storage
oscilloscope till reaching the melting point and the lamp burned-out then. If the burnout
profile [61] didn’t include filament breakdown and showed only support melting as shown in
figure 12 , then the measurement must be repeated with another lamp brand with thicker
support stems to ensure attaining the tungsten melting temperature.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
13
Figure 12. Close-up showing different type of filament lamp samples burnout near melting temperature of
tungsten.
All vibration patterns were analyzed by standard Microsoft Office Excel 2010 FFT analysis
tool with resolution of 1024 channels to obtain the frequency spectrum of the filament at
each temperature.
Results and Discussion
As seen in figure 13a, the vibration pattern of the tungsten filament at room temperature
shows a very long damping time that lasts for several seconds. The time constant is 1.25 s,
the quality factor of the oscillation is 3333 and hence, the internal friction is approximately
0.0003. The dominant oscillation wave form as seen in figure 13b, is sinusoidal which means
that the oscillation mode is purely simple longitudinal.
(a) (b)
Figure 13. Oscilloscope picture for the filament impulse vibration pattern at room temperature after a 5ms
solenoid plunger pulse at different time scales (a) the damping pattern at 500ms /division. (b) The oscillation
waveform at center amplitude at 1ms /division.
the vibration pattern of the tungsten filament near melting temperature shows a very short
damping time that lasts for a fraction of second as seen in figure 14. The time constant is
0.1s, the quality factor of the oscillation dropped to 129.8 and hence, the internal friction
increased to 0.0077 which is 25 times greater than that of room temperature The dominant
oscillation wave form as seen in figure 14b, isn’t any more sinusoidal which means that the
oscillation mode my contain higher harmonics or different modes.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
14
(a) (b)
Figure 14. Oscilloscope picture for the filament impulse vibration pattern at 3300 o C after a 5ms solenoid
plunger pulse at different time scales (a) the damping pattern at 500ms /division. (b) The oscillation waveform
at 1ms /division.
If we study the frequency spectrum of the filament impulse response at room temperature as
shown in figure 15a, we notice a single longitudinal vibration at 833Hz (denoted 1) and its
symmetric complement at 27HZ that arises because of the double side band signal (DSB)
pattern. All symmetric complements are ignored. As the filament temperature continue to
increase, it began to lose its stiffness and it may sag under the effect of gravity. At this limit
the excitation pulse induces several transversal modes of vibration. Figure 15b shows the
filament impulse response at near melting temperature of tungsten, where the main
longitudinal frequency mode (denoted 1) was decreased in magnitude and similarly in
frequency to 411Hz. Several strong transversal modes tested by autocorrelation (denoted 2, 3,
4) are also present.
(a) (b)
Figure 15. Symmetric DSB FFT spectrogram for (a) Room temperature impulse pattern of the filament. (b)
Near melting temperature impulse pattern of the filament.
Now, If we plot the applied voltage versus the filament current data as shown in figure 16a
we notice a very smooth curve leading to the calculation of filament temperature by using
equation 19. Then we can plot the main longitudinal frequency versus filament current as
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
15
shown in figure 16b, to obtain the filament resonance frequency versus its temperature as
shown in figure 17a.
(a) (b)
Figure 16. Filament current versus (a) The applied voltage across filament terminals (b) Filament natural
frequency.
Tests revealed that the elastic moduli of tungsten decrease as the temperature of the sample
increases till the molting point on three steps. At first a slow decrease in elasticity moduli in
the temperature range from room to 1000oC is observed, followed by an accelerated decrease
till 2600oC, then suddenly drops to 20% of its initial value just below melting point. The
reason behind this behavior may be ought to α and β crystalline phase transition of tungsten
occurring at the edges of thermal slope inflections. Both Young and bulk moduli tends to
intercept at melting point. This could be explained easily in light of symmetry anisotropy
caused by crystalline zones melting.
(a) (b)
Figure 17. Filament temperature versus (a) Filament natural frequency. (b) The elasticity moduli of the
filament non-sag tungsten.
A remarkable enhancement and decreased of end-loss thermal gradient along the filament
length L , is noticed after exceeding a temperature of 800oC as revealed by direct filament
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
16
photography shown in figure 18. Simultaneously, both the natural frequency of the filament
and its vibration damping pattern time constant is decreased as the temperature increased as
illustrated in the same figure. This decrease is due to the increase in tungsten internal friction
as function of temperature [28] which may be described in a separated work.
Figure 18. Tungsten filament linear incandescence, natural frequency and impulse damping resonance pattern
at different temperatures
Figure19. represents the normalized tungsten filament resistance versus the normalized
resonance frequency showing a second order best fit curve. At near melting point the filament
resistance is twenty times its room temperature value and the Young's modulus is one fifth its
initial value and Hence the elasticity of tungsten is increased five folds at this extent.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
17
(a) (b)
Figure 19. Normalized regression of (a) Tungsten filament resistance versus Young’s modulus (b) Tungsten
filament natural frequency versus Young’s modulus.
Figure 21a shows the tungsten elasticity moduli as a function of temperature obtained by our
work and compared to data calculated using the results of reference [23]
(a) (b)
Figure 20. (a) Elasticity moduli of tungsten obtained in this work compared to those calculated according to the
result of reference [23] (b) Deviation percent of the young’s modulus results from those of reference [23].
We found that, instead of equation 1, our experimental dynamic Young’s modulus results
may be better represented by a third order best-fit parametric equation on the form:
( )
(24)
Where T ranges from 27oC to 3400
oC covering the whole range from room temperature to
near melting point of tungsten. The value the regression constants ao, a1 , a2 and a3 are given
in Table 4.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
18
Table 4. Comparison between the coefficients of parametric regression equations for the Young’s modulus
experimental data obtained by laser Doppler vibrometry and laser shadowgraphy- based vibrometry.
Regression coefficients
For the results of reference [] in the
range from 27-2650oC
0
For the results of the present work in
the range from 27-3400oC
Conclusion
Changing the symmetry of the tungsten sample from wire string to helical coil in impulse
excitation technique, enhances the dynamic elasticity moduli measurements. This
enhancement is due to the minimization of temperature gradient over the sample length and
decrease the end-loss. Similarly, changing the sample heating method from pulsed current to
direct current also eases the measurement and exclude pyrometry from the measurement
procedure. The use of shadowgraphy based vibrometry assisted by lock-in photo-detection
technique enable low cost measurements, while increasing sample temperature to near
melting point. Experimental tests on commercial grade non-sag tungsten filament of P21W
lamp, leads to an exclusive third order parametric equation describing the Young’s modulus
of tungsten from 27oC to 3400
oC measured for the first time. The obtained data is compared
to those obtained by laser Doppler vibrometry and pulsed current heating method up to
2650oC. An agreement between the yield of both method with only 15% maximum deviation
due to the effect of sample impurities on thermo-elastic behavior in our sample and the high
thermal gradient of the reference sample. The main finding of our work is, the 5 folds
decrease in tungsten Young’s modulus was noticed near tungsten melting point as well as the
25 folds increase in internal friction. The method described in this work may be used as non-
contact in-plan vibrometry tool for studying vibration of incandescent objects, unlimited by
their surface emissivity or roughness. This method may help in the future synthesis and test
of new grade of refractory materials, deployed as plasma facing material in the latest fusion
reactor or super alloys in critical applications subject to extreme temperature.
Acknowledgment
The authors are very grateful to the members of Laser Research Technology Center,
Engineering Physics Department, Military Technical College, Cairo, Egypt and Physics
Department, Faculty of Science, Cairo University and for their support with measurement
instruments, encouragement and helpful suggestions.
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
19
References
[1] Aldazabal, J., C. García-Rosales, A. Martín Meizoso, N. Ordás, F. Sordo, J. L. Martínez, and J. Gil
Sevillano. "A comparison of the structure and mechanical properties of commercially pure tungsten
rolled plates for the target of the European spallation source." International Journal of Refractory
Metals and Hard Materials 70 (2018): 45-55.
[2] Meng, QingLing, LiangLiang Niu, Ying Zhang, and GuangHong Lu. "Molecular dynamics
simulations of temperature effect on tungsten sputtering yields under helium bombardment." Science
China Physics, Mechanics & Astronomy 61, no. 1 (2018): 017121.
[3] Litnovsky, A., T. Wegener, F. Klein, Ch Linsmeier, M. Rasinski, A. Kreter, B. Unterberg et al.
"Smart tungsten alloys as a material for the first wall of a future fusion power plant." Nuclear Fusion
57, no. 6 (2017): 066020.
[4] Marian, J., C. S. Becquart, C. Domain, S. L. Dudarev, M. R. Gilbert, R. J. Kurtz, D. R. Mason et al.
"Recent advances in computational materials modeling of tungsten as plasma-facing material for
fusion energy applications." Nucl. Fusion 57 (2017).
[5] Koyanagi, Takaaki, NAP Kiran Kumar, Taehyun Hwang, Lauren M. Garrison, Xunxiang Hu, Lance
L. Snead, and Yutai Katoh. "Microstructural evolution of pure tungsten neutron irradiated with a
mixed energy spectrum." Journal of Nuclear Materials 490 (2017): 66-74.
[6] osemann, P., D. Frazer, M. Fratoni, A. Bolind, and M. F. Ashby. "Materials selection for nuclear
applications: Challenges and opportunities." Scripta Materialia (2017).
[7] Igor L. Shabalin, Ultra-High Temperature Materials I: Carbon (Graphene/Graphite) and refractory
metals, springer science + business media Dordrechet (2014) ISBN 978-94-007-7586-2.
[8] Lassner, Erik, and Wolf-Dieter Schubert. Tungsten: properties, chemistry, technology of the element,
alloys, and chemical compounds. Springer Science & Business Media, 2012.
[9] Kaufmann, M., and R. Neu. "Tungsten as first wall material in fusion devices." Fusion Engineering
and Design 82, no. 5 (2007): 521-527.
[10] Neu, R., R. Dux, A. Kallenbach, T. Pütterich, M. Balden, J. C. Fuchs, A. Herrmann et al. "Tungsten:
an option for divertor and main chamber plasma facing components in future fusion devices."
Nuclear fusion 45, no. 3 (2005): 209.
[11] Alan Wolfenden (Ed), Dynamic Elastic Modulus Measurements in Materials, Issue 1045 Publisher
ASTM International (1990) ISBN 0803112912, 9780803112919,.
[12] R. Pendleton, M. Tuttle, Manual on Experimental Methods for Mechanical Testing of Composites,
Springer Science & Business Media, (2012) ISBN 9400911297, 9789400911291.
[13] Standard test method for dynamic Young’s modulus, shear modulus and Poisson ratio for advanced
ceramics by impulse excitation of vibration ASTM designation: C1259-95, 1995, pp. 375.
[14] Acsente, Tomy, Raluca Florentina Negrea, Leona Cristina Nistor, Constantin Logofatu, Elena Matei,
Ruxandra Birjega, Christian Grisolia, and Gheorghe Dinescu. "Synthesis of flower-like tungsten
nanoparticles by magnetron sputtering combined with gas aggregation." The European Physical
Journal D 69, no. 6 (2015): 161.
[15] Khani, Arash Hadavand, A. M. Rashidi, and Giti Kashi. "Synthesis of tungsten nanoparticles by
reverse micelle method." Journal of Molecular Liquids 241 (2017): 897-903
[16] Sarmah, Trinayan, Ngangom Aomoa, G. Bhattacharjee, Sidananda Sarma, Biswajit Bora, D. N.
Srivastava, H. Bhuyan, M. Kakati, and G. De Temmerman. "Plasma expansion synthesis of tungsten
nanopowder." Journal of Alloys and Compounds 725 (2017): 606-615.
[17] Enneti, Ravi K. "Synthesis of nanocrystalline tungsten and tungsten carbide powders in a single step
via thermal plasma technique." International Journal of Refractory Metals and Hard Materials 53
(2015): 111-116.
[18] Zhou, Le, Frank Kellogg, Clara Hofmeister, Anit Giri, Kyu Cho, and Yongho Sohn. "Nanostructured
tungsten through cryogenic attrition." International Journal of Refractory Metals and Hard Materials
52 (2015): 70-77.
[19] Periyannan, S., and K. Balasubramaniam. "Moduli determination at different temperatures by an
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
20
ultrasonic waveguide method." Experimental Mechanics 56, no. 7 (2016): 1257-1270.
[20] Tillmann, W., U. Selvadurai, and W. Luo. "Measurement of the Young’s modulus of thermal spray
coatings by means of several methods." Journal of thermal spray technology 22, no. 2-3 (2013): 290-
298.
[21] Richards, J.T., "An Evaluation of Several Static and Dynamic Methods for Determining Elastic
Moduli," Symposium on Determination of Elastic Constants, Special Technical Publication No. 129
of The American Society for Testing Materials, 25 June 1952.
[22] Periyannan, Suresh, and Krishnan Balasubramaniam. "Simultaneous moduli measurement of elastic
materials at elevated temperatures using an ultrasonic waveguide method." Review of Scientific
Instruments 86, no. 11 (2015): 114903.
[23] Škoro, G. P., J. R. J. Bennett, T. R. Edgecock, S. A. Gray, A. J. McFarland, C. N. Booth, K. J.
Rodgers, and J. J. Back. "Dynamic Young’s moduli of tungsten and tantalum at high temperature and
stress." Journal of Nuclear Materials 409, no. 1 (2011): 40-46
[24] Štubňa, Igor, Anton Trník, and Libor Vozár. "Determination of Young's modulus of ceramics from
flexural vibration at elevated temperatures." Acta Acustica united with Acustica 97, no. 1 (2011): 1-
7.
[25] Kogo, Yasuo, Yoshie Iijima, and Naohiro Igata. "Internal friction of carbon–carbon composites at
elevated temperatures." Journal of alloys and compounds 355, no. 1 (2003): 148-153.
[26] Dandekar, Dattatraya P., and Anthony G. Martin. "Temperature dependence of flexural and torsional
elastic constants of two nickel-based superalloys." Journal of Materials Science 25, no. 7 (1990):
3321-3326
[27] Ashkenazi, J., M. Dacorogna, M. Peter, Y. Talmor, E. Walker, and S. Steinemann. "Elastic constants
in Nb-Zr alloys from zero temperature to the melting point: Experiment and theory." Physical
Review B 18, no. 8 (1978): 4120.
[28] I. BERLEC, "The effect of impurities and heat treatment on the internal on the internal friction of
Tungsten at high temperatures", Metallurgical Transactions, 1, 2677-2683, 1970.
[29] Varshni, Y. P. "Temperature dependence of the elastic constants." Physical Review B 2, no. 10
(1970): 3952.
[30] JW Neudecker, CR Sanders, Young's Modulus Measurements to 2500'C by the Thin-Rod
Resonance Technique. Advances in Instrumentation. Vol. 24, pt. 2 - Inst. SOC. Am, 1969.
[31] Armstrong, Philip E. ; and Brown, Harry L. : Dynamic Young's Modulus Measurement Above 1000°
C on Some Pure Polycrystalline Metals and Commercial Graphites. Trans. AIME, vol. 230, no. 5,
Aug. 1964, pp. 962-966.
[32] Robinson, S. L., and O. D. Sherby. "Mechanical behavior of polycrystalline tungsten at elevated
temperature." Acta Metallurgica 17, no. 2 (1969): 109-125.
[33] Carnevale, Edmund H. "Acoustic techniques and applications at elevated temperatures." NASA
Special Publication 132 (1967): 73.
[34] Lowrie, Robert; Gonas, A. M. Single crystal Elastic Properties of Polycrystalline Tungsten, 24°-
1800°C, Journal of Applied Physics, 38, 7, p.4505-4509 (1967).
[35] Lytton, Jack L., John A. Hren, Kenneth T. Kamber, and Oleg D. Sherby. "Apparatus for the
determination of dynamic Young's modulus and internal friction in vacuum at temperatures from 25°
C to 1200° C." British Journal of Applied Physics 15, no. 12 (1964): 1573.
[36] Brown, Harry L., and Philip E. Armstrong. "Young's Modulus Measurements above 2000° C."
Review of Scientific Instruments 34, no. 6 (1963): 636-639.
[37] W. Hl. Hill, K. E. Shimmin, Elevated Temperature Dynamic Elastic Moduli Of Various Metallic
Materials, MATERIALS CENTRAL,Wright Air Development Division, Wadd Technical REPORT
60-13874, 1961.
[38] Fine, M.E., "Dynamic Methods for Determining the Elastic Constants and their Temperature
Variation in Metals," Symposium on Determination of Elastic Constants Special Technical
Publication No. 129 of the American Society for Testing Materials, 25 June 1952.
[39] Hill, W. H., and K. D. Shimmin. Elevated temperature dynamic elastic moduli of various metallic
materials. METAL HYDRIDES INC BEVERLY MA, 1961.
[40] Lees, Chas H., Jas P. Andrews, and L. S. Shave. "The variation of Young's modulus at high
Military Technical College
Kobry Elkobbah,
Cairo, Egypt
April 3-5,2018
9th International Conference
on Mathematics and
Engineering Physics
(ICMEP-9)
21
temperatures." Proceedings of the Physical Society of London 36, no. 1 (1923): 405.
[41] Andrews, Jas P. "The variation of Young's Modulus at high temperatures." Proceedings of the
Physical Society of London 37, no. 1 (1924): 169.
[42] Agrawal, D. C. "The Coiling Factor in the Tungsten Filament Lamps." Lat. Am. J. Phys. Educ. Vol
5, no. 2 (2011): 443.
[43] Halas, S. and Durakiewicz, T.,. Temperature distribution along a metal filament heated in vacuum by
DC current. Vacuum, 49(4), pp.331-336. (1998)
[44] Jain, S. C., and K. S. Krishnan. "The Distribution of Temperature along a Thin Rod Electrically
Heated In vacuo. IV. Many Useful Empirical Formulae Verified." In Proceedings of the Royal
Society of London A: Mathematical, Physical and Engineering Sciences, vol. 225, no. 1160, pp. 19-
32. The Royal Society, 1954.
[45] Prins, J. A., J. Schenk, and J. M. Dumoré. "Temperature distribution at the end of a hot wire."
Applied Scientific Research 3, no. 4 (1952): 272-278.
[46] Worthing, A. G. "Theory of end-loss corrections and its application to uniform, electrically heated
tungsten filaments in vacuo." Journal of the Franklin Institute 194, no. 5 (1922): 597-611.
[47] Langmuir, Irving. "The characteristics of tungsten filaments as functions of temperature." Physical
Review 7, no. 3 (1916): 302.
[48] J. Vass, R. Smid, R.B. Randall, P. Sovka, C. Cristalli, B. Torcianti, Avoidance of speckle noise in
laser Vibrometry by the use of kurtosis ratio: Application to mechanical fault diagnostics,
Mechanical Systems and Signal Processing 22, 647-671, 2008.Castellini, M. Martarelli, E.P.
[49] Tomasini, Laser Doppler Vibrometry: Development Of Advanced
Solutions Answering to Technology’s needs, Mechanical systems and Signal Processing 20, 12 -
1285, 2006.
[50] A. M. Wahl, Mechanical Springs, 2nd Edition, McGraw-Hill, Inc., New York, 1963.
[51] Gere, James M. "Mechanics of Materials, th 5 ed." USA: Brooks/Cole (2001).
[52] D. C. Agrawal, V. J. Menon, "Light bulb exponent-rules for the classroom", IEEE Transactions on
Education, 43, 262-265, 2000.
[53] E. G. Wolff, Measurement Techniques for Low Expansion Materials, 9th National SAMPE
Technical Conference, AtlantaGa, 9, 57-72, 1977.
[54] Monier, Romain, François Thumerel, Julien Chapuis, Fabien Soulié, and Cyril Bordreuil. "Liquid
metals surface temperature fields measurements with a two-colour pyrometer." Measurement 101
(2017): 72-80
[55] Cadar, Sergiu, Dorin Petreuş, Etz Radu, Frenţiu Tiberiu, Darvasi Eugen, and Sanziana Butaciu.
"Temperature and power consumption for tungsten coil in the drying process of liquid samples." In
Electronics Technology (ISSE), 2016 39th International Spring Seminar on, pp. 348-352. IEEE,
2016.
[56] H.H. Hassan, S.A. Khairy and H.S. Ayoub, A Simple Laboratory Experiment for Measuring the
Expansivity of Tungsten at Elevated Temperatures, Nature and Science; 13(11), 146-151, 2015.
[57] Dauphin, M., S. Albin, M. El Hafi, Y. Le Maoult, and F. M. Schmidt. "Towards thermal model of
automotive lamps." In 11th International Conference on Quantitative InfraRed Thermography. 2012
[58] Sobczyk, Zbigniew. "Total current measurement interrupts detection method in automotive bulbs
circuits." Journal of KONES 18 (2011): 579-584.
[59] De Izarra, Charles, and Jean-Michel Gitton. "Calibration and temperature profile of a tungsten
filament lamp." European Journal of Physics 31, no. 4 (2010): 933.C.
[60] Calzà, G., L. M. Gratton, T. López-Arias, and S. Oss. "Very fast temperature measurement with a
thin lamp filament." Physics Education 47, no. 3 (2012): 334.
[61] Gluck, Paul, and John King. "Physics of incandescent lamp burnout." The Physics Teacher 46, no. 1
(2008): 29-35.